International Journal of Engineering Science Invention ISSN (Online): 2319 – 6734, ISSN (Print): 2319 – 6726 www.ijesi.org Volume 2 Issue 12ǁ December 2013 ǁ PP.59-69

A Study of Zenner – Holomon Parameter Variation with Pass Reduction in Steel Rolling 1,

Okediran, I.K., 2,Alamu, O.J. and 3,Durowoju, M.O.

Department of Mechanical Engineering, Osun State University, Osogbo, Nigeria.

ABRSTRACT : An attempt is made in this work to establish mathematical relationships between the Zener – Hollomon Parameter and rolling reduction per pass in the hot rolling of Type 316 High Carbon Stainless Steel (HCSS316). The hot rolling simulation of steel based on the Reverse Sandwich Model and that based on the Sims‟ theory were used with the hot rolling experimental data for HCSS316, to generate results which reveal the dependency of the two rolling parameters on each other. These results were then processed with the EXCEL Package to arrive at a quantitative description of the observed relationship. The Zener–Hollomon parameter (Z) was found to be a non linear function of rolling reduction (r): ( Log 10Z ar br cr d ;...... a, b, c, d cons tan ts ) for High Carbon Stainless Steel hot flat rolled at low strain rates. The results compare favourably with experimental inferences. 3

2

KEY WORD: Zener-Hollomon Parameter, rolling reduction, simulation] I.

INTRODUCTION

Rolling nowadays accounts for about 90% of all metals produced by metal working processes. It was first developed in the late 1500s. Traditionally, the initial material form for rolling was an ingot. By far the largest amount of finished steel production is achieved by rolling. The Semi-finished products cast from the steelmaking furnace are reheated to the austenising range and passed through a series of mills with rolls of the required profile to force the hot steel into the finished shape. (Graham, 1993) Developed in the mid – 1800s two high and three high rolling mills are still used today for initial breakdown passes on cast ingots. However, this practice is now being rapidly replaced by continuous casting and rolling, with much higher efficiency and lower cost.The advent of continuous casters has necessitated hot flat rolling at low strain rates (0.01 – 1.55) s-1 and low reduction ( 10%) (Aiyedun, 1986). Under such rolling condition, the contact time in the roll gap increases and heat loss from the pre-heated ingot to the surroundings and the rolls increases. This variation in temperature induces a non-uniform deformation pattern in the through-thickness of the rolled steel. The deformation, by virtue of the un-even re-crystallization and grain refinement, as a result creates in the material a low-temperature harder surface and a high-temperature softer core (Alamu and Aiyedun, 2003, Ojediran and Alamu, 2003).(see Fig.1)The prevailing situation has been investigated by authors. Barbosa, (1983), Leduc, (1983), and Aiyedun (1984) referred to the observed effect as “Reverse Sandwich” or Roll chilling, as the through-thickness hardness variation presents a direct opposite of what obtains in a sandwich rolling process, where harder metals are sandwiched between layers of softer metals to effect rolling of very hard and high strength metals into thin strips without rupture in the rolls (Afonja and Sansome, 1973). Studies abound in literatures on deformation in sandwich rolling and the reverse sandwich effect or roll chilling. The adoption of computer simulation in modeling engineering systems further expands this area of study. The Zener-Hollomon parameter is uniquely related to stresses, and gives an indication of deformation in a material. Researchers (Zener and Hollomon, 1944; Aiyedun, 1984) have long established that deformation increases with decreasing Zener – Hollomon parameter value. Alamu and Taiwo, (2002) employed computer simulation to study deformation pattern in the hot rolling of High Carbon Stainless Steel type 316 (HCSSS316) using a reverse Sandwich Model developed by Shobowale (1998). In the work, the reverse sandwich model was simulated incorporating strain rate and Zener-Hollomon parameter computation for different zones along the thickness of HCSS316 during hot flat rolling, thus permitting a study of the deformation pattern of this material during hot rolling.In this work, the relationship between deformation rate, in terms of the Zener-Hollomon parameter and rolling reduction per pass in the hot rolling of HCSS316 is investigated, using the reverse sandwich model and Sims‟ theory of hot flat rolling, with hot flat rolling experimental data earlier obtained by researchers for HCSS316.

www.ijesi.org

59 | Page

A Study Of Zenner – Holomon Parameter Variation…

II. MATERIALS AND METHOD Deformation in hot rolling is temperature dependent. In this process the strength of a metal decreases as temperature rises, and its grains can be distorted more easily. In line with Sims‟ theory, hot rolling process is characterized by “sticking throughout the roll gap” (Sims, 1954). However, this is not entirely true for hot rolling of HCSS316 at low strain rates; here, the rolling surfaces are sufficiently chilled leading to a mixed sliding –sticking condition in the roll gap (Aiyedun, 1986).

THEORIES OF METAL ROLLING Lennard (1980), and Usamah and Lennard (1980), amongst other literatures have reported that, Orowan‟s theory is the most comprehensive among the many theories of rolling. According to Lennard, (1980), the approach requires mathematical descriptions of material behaviour and deformation as well as assumptions of frictional conditions at the roll – metal interface and mode of roll deformation. The complexity of the method of solution of Orowan‟s equation caused later researchers, notably, Sims, Bland and Ford, Alexander, Alexander and Ford and Atreya and Lennard to develop solutions based on simplifying assumptions. 1.

Orowan’s Theory: According to Lennard, (1980) Orowan‟s theory can be summarized in the differential equation:

d hs 2k tan 2 R`s.sin cos d where:

……………..

(1)

interfacial shear stress, roll pressure, thickness of the strip in the roll gap, yield strength in shear of the material, current radius of curvature of the roll at a particular location, independent variable (angle) measured from the centre line in the roll gap. The instantaneous yield stress, k, depends on rolling temperature, strain and strain rate, and must be determined s h k R`

= = = = = =

before evaluating the mean yield stress, K , for subsequent computation of rolling parameters of interest such as load and torque. 2.

Sims’ Theory of Hot Flat Rolling:

According to Sims (1954), the only practicable method of allowing for the elastic deformation of the rolls is that due to Hitchcock, who replaced the actual distribution of pressure over the roll surface with an elliptical distribution giving the same total load. The roll, in its arc of contact with the material, is then of constant radius of curvature. Sims‟ hot flat rolling theory assumes a circular arc of contact, which is flattened in accordance with Hitchcok‟s formular:

C .P R` Ro1 .W

……………………………… (2)

where: R‟ = radius of curvature of the elastically deformed roll, (mm) Ro = un-deformed roll radius, (mm), P = vertical roll pressure, (N/mm2 ) W = width of the material, (mm), C = constant, and,

C 8

1 v 2

E

…………………………………(3)

also,

= 0.0223 mm2 kN-1 for steel rolls, = 0.0247 mm2 kN-1 for chilled C.I. rolls 2 P =132KN/ mm (Sims, 1954; Aiyedun, 1984) However, several authors have questioned the validity of this approach.

3.

The Bland and Ford’s Theory:

The Bland and Fords theory is basically a theory for cold rolling, where sliding takes place throughout the arc of contact but has been found applicable to hot rolling of HCSS316, where there is a mixed sticking - sliding condition (Aiyedun 1984). This is the situation for hot rolling of HCSS316 at (900 – 1200)oC, (0 – 15) % reduction, (0.07 – 1.5) s-1 strain rates.

www.ijesi.org

60 | Page

A Study Of Zenner – Holomon Parameter Variation… THE ROLL CHILLING EFFECT A detailed description of the Reverse Sandwich Model based on the „Roll Chilling Effect‟, which characterizes hot rolling of HCSS316 has been presented elsewhere; (Shobowale, (1998), Alamu, (2001), Alamu and Aiyedun, (2003)). The reverse sandwich rolling presents a situation whereby a high strength - metal clads a low strength metal. The strength variation being a direct consequence of drastic temperature changes during rolling. The reverse sandwich model predicts rolling temperatures, temperature distribution corresponding to different heights (17 Zones), the Zener-Hollomon parameter, yield stresses, rolling load and torque for HCSS316 rolled at low strain rates and low reduction. DEFORMATION IN MATERIAL AND ROLLING TEMPERATURE Extensive research work has been carried out on deformation modeling using the Zener-Hollomon parameter. A general drop in the Zener-Hollomon parameter from the rolling surfaces (lowest temperature zone) towards the core (temperature peak) of the material was observed by Alamu and Taiwo, (2002), implying that the material deforms increasingly towards the centre. The conclusion drawn was corroborated with the fact that metals deform at a greater rate at elevated temperatures (Early, 1977) PASS REDUCTION AND THE ZENER – HOLLOMON PARAMETER Reduction per pass during metal rolling process is given as: ……………………………………. (4) Hf Ho where; = rolling reduction, (mm), Hf = final specimen thickness, (mm), Ho = initial specimen thickness, (mm). Expressed as a percentage, we have:

r

Hf Ho 100% Ho

…………………………………… (5)

The Zener-Hollomon parameter was determined using the proposition of Zener and Hollomon, (1944):

Q

f exp f (Z ) RT

……………………. (6)

= strain rate R = universal constant, (J /mol..K), T = absolute temperature, (OC) Z = Zener-Hollomon parameter. Q = energy supplied by the thermal fluctuation to overcome obstacles such as dislocations. The Z-values are uniquely related to the stress, and, hence the deformation of the material. For HCSS316 at (900 – 1200)oC, (0 – 15) % reduction, and (0.07 – 1.5) s-1 strain rates, Q = 460kJ / mol (Aiyedun, 1984). where;

III.

MEAN STRAIN RATE

The resistance to deformation of hot metal is both strain and strain rate dependent. For this reason it is necessary to define the mean strain rate in the rolling pass. According to Orowan and Pascal, mean strain rate is given as;

Vn Rh1

1 34 r r 1 r

…………………………(7)

where; = rolling velocity at the neutral position. Vn Ford and Alexander expressed it in the form:

Vn Rh1

4 3r r 2 2 r

…………………..(8)

The form of mean strain rate estimation adopted by Sims, R. B. is given as:

Vn

1 ln r 1 r

1

Rh1

……………………(9)

Integration of equation (9) into equation (6) above gives the basis of Zener – Hollomon Parameter computation adopted by Sims. (Aiyedun, (1984) According to Sellars, (1981) instantaneous strain rate in the roll gap is

2v

h1 h 2 0.5 R 0 .5 h

www.ijesi.org

……………………(10)

61 | Page

A Study Of Zenner – Holomon Parameter Variation… He further stated that the best mean strain rate will be one that gives a correct mean flow stress. Farag and Sellars, (1973) thus obtained an approximate empirical equation of the form: 0.25 h1 0.45 1.08V 2 ln 0.5 0.5 R` h1h 2 h 2

……………………………… (11)

where: = reduction V = peripheral velocity of rolls (mms -1) The above equation due to Farag and Sellars was adopted in the Reverse Sandwich Model for computation of mean strain rate, which was then used in equation (6) to estimate the Zener - Hollomon Parameter (The quantity used to model deformation).

IV. MODEL SIMULATION AND VALIDATION The computer code developed using FORTRAN 77 for Zener - Hollomon Parameter computation at different rolling reduction using the Reverse sandwich model is as provided. Fig. 2 shows the flow chart for the simulation. The Program is user friendly and interactive, accepting input manually from the screen and outputting results to user-defined file. Validation of the program was accomplished using data from hot rolling experimental work carried out by authors on HCSS316 using 2 high reversing laboratory rolling mills. For the material under study, experimental data abound in literatures for hot rolling based on Sims‟ theory of hot flat rolling (Aiyedun, 1984; Shobowale, 1998; Alamu, 2001). The composition and thermo-mechanical history of the specimen is presented in Table I, while the input data for the simulation is as shown in Table II.

V.

RESULTS AND DISCUSSION

The Output of the computer program, run with an IBM compatible Pentium (r) Processor, is presented in Tables III - VI. The tables show the Zener – Hollomon Parameter values corresponding to different rolling reduction characterized in different specimen. Also, the tables present the mean rolling temperature for each hot rolling schedule to enable further validation of the program via a comparison between simulated and experimental mean temperatures. This comparison is presented in Fig. 4. Similar data, from literatures, for hot flat rolling of HCSS316 adopting Sims‟ theory is presented in Table VII. These sets of data, processed with EXCEL package gave the polynomials shown in Fig. 3From the tables, variation of the Zener – Hollomon Parameter with rolling reduction is evident. This is in agreement with earlier works of authors (Shobowale, 1998; Alamu and Taiwo, 2002). In other words, the rate of deformation in HCSS316 during hot rolling is a function of the rolling reduction per pass. The possible relationship between these two parameters, as evident in Fig. 3, takes the form of a non-linear polynomial, and is consistent in the two approaches; the Reverse sandwich Model and Sims‟ theory. From the two approaches investigated, the Zener – Hollomon Parameter as a function of rolling reduction takes

the form: ( Log 10Z ar br cr d ;...... a, b, c, d cons tan ts ). For Sims‟ theory, a = -0.1833, b = 1.45, c = -2.8667, d = 21; while for Reverse Sandwich Model; a = 0.1367, b = -1.28, c = 3.9833, and, d = 16.82. 3

2

Fig. 4 reveals an agreement between simulated mean temperature and experimental values. Similar comparisons have been used in other works (Shobowale, 1998; Alamu and Aiyedun, 2002, Ojediran and Alamu, 2002) to confirm the validity of the output of the computer program. Hence, results obtained compares favourably with experimental inferences as well as earlier works of researchers.

VI.

CONCLUSION

In the hot rolling of HCSS316 at low strain rates, (0.01 – 1.55) s-1 and low reductions, ( 10%), the Zener – Hollomon Parameter, (Z), has been found to be dependent on rolling reduction, (r), per

pass. For Sims‟ theory, Log 10Z 0.1833 r 1.45 r 2.8667 r 21 ; while using the Reverse 3

2

sandwich Model, Log 10Z 0.1367 r 1.28 r 3.9833 r 16 .82 for hot rolling computations. 3

2

www.ijesi.org

62 | Page

A Study Of Zenner – Holomon Parameter Variation…

[1] [2] [3] [4]

[5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18]

REFERENCES Afonja, A. A. and Sansome, D. H. (1973), “A Theoretical Analysis of the Sandwich Rolling Process” Int. J. Mech. Sci., 15 (1): 1 – 14. Aiyedun, P. O. (1984) “A Study of Loads and Torques for Light Reduction in Hot Flat Rolling” Ph. D. Thesis, University of Sheffield. Aiyedun, P. O. (1986), “Hot Flat Rolling Simulation by Use of the Bland and Ford‟s Cold Rolling Theory for HCSS316 at Low Reduction and Low Strain Rates”, Proc, Int. AMSE Conf., 3 (1): 14 – 36. Alamu, O. J. (2001) “Integration of the Reverse Sandwich Model into the Hot Rolling Bland and Ford‟s Theory for Load and Torque Calculations”, M. Sc. Project Report, University of Ibadan, Ibadan, Nigeria. Alamu, O. J. and Aiyedun, P. O. (2003) “A Comparison of Temperature Gradient in Hot Rolling at Low and High Strain Rates” JSET, 10 (1) (In Press) Alamu, O. J. and Taiwo, A. “Computational Approach to a Study of Deformation in HCSS316 During Hot Rolling, The Nigerian Academic Forum, (In Press) Barbosa, R. A. N. M., (1983), Ph. D. Thesis, University of Sheffield. Early, J.G. (1977) “Elevated Temperature Mechanical Behaviour of a Carbon-Manganese Pressure Vessel Steel” Journal of Engineering Materials and Technology, pp. 359 – 365. Farag, M. M. and Sellars, C. M., (1979) “Hot Working and Forming Process”, Paper presented at Metals Society Conference, Sheffield. Graham, W. O., Peter, R. K. and Partrick, J. D. (1993) Steel Designer‟s Manual, 5th ed. Blackwell Scientific Publishers, London Leduc, L. A., (1980), Ph. D. Thesis, University of Sheffield. Lenard, J.G. (1980) “Roll Deformation in Cold Strip Rolling” Journal of Engineering Materials and Technology, 102 (1):382 – 383. Ojediran, J. O and Alamu, O. J (2002) “A study of Core Temperature Characteristics of Hot flat Rolled HCSS 316” International Journal of Research in Science and Education 2(2) Sellars, C. M. (1981) Paper presented at Colloque de Metallurgie, Institut National des Science et Technique Nucleaires, Sanclay. Shobowale, B. (1998) “The Reverse Sandwich Effect in HCSS316 Hot Flat Rolled at Low Strain Rates and Low Reductions”, M. Sc. Project Report, University of Ibadan, Ibadan, Nigeria. Sims, R.B. (1954) “The Calculation of Roll Force and Torque in Hot Rolling Mills” J.I.S.I. Pp. 191 – 200. Usamah, S. and Lenard, J. G. (1980) “A Comparison of Cold Rolling Theories Based on the Equilibrium Approach” Journal of Engineering Materials and Technology, 102 (1): 223 – 228. Zener, C. and Hollomon, J.H., (1944), Journal of Applied Physics, 15, 22.

C------------------------------------------------------------------C Program : HOT ROLLING DEFORMATION BASED ON RSM MODEL C___________________________________________________________________ IMPLICIT REAL*8(A-H,O-Z) DIMENSION T(17),H(17),PLOT(17) CHARACTER RSM*20, SPNO*6,CONTD DATA IN/'N'/,IY/'Y'/ Q=460000.0 GKR=8.314 P=132.0 C=0.02474 RO=139.70 AZEN = 0.0 C

FILES CREATION AND INTERACTIVE DATA ENTRY WRITE(*,*)'Enter a Filename for the Result.' READ(*,25)RSM OPEN(UNIT=7,FILE=RSM,STATUS='NEW')

10 WRITE(*,*)'Supply the Specimen Identification Number.' READ(*,12)SPNO

www.ijesi.org

63 | Page

A Study Of Zenner – Holomon Parameter Variation… WRITE(*,*)'Enter the Rolling Speed,(mm/s).' READ(*,*)V WRITE(*,*)'Supply the Furnace Temperature (Deg.Celcius).' READ(*,*)TF WRITE(*,*)'Supply the Initial Specimen Height,(mm).' READ(*,*)HO WRITE(*,*)'Enter the Final Specimen Height,(mm).' READ(*,*)HF WRITE(*,*) 'Enter the Width of the Specimen,(mm).' READ(*,*) W WRITE(7,*) WRITE(7,100)SPNO 100 FORMAT(1X,'OUTPUT FOR SPECIMEN 'A4) WRITE(7,*)'------------------------------------------' 12 FORMAT(A4) 20 FORMAT(A1) 25 FORMAT(A4) C RELATIONSHIP BETWEEN ROLLING SPEED(V) AND THE REVERSE SANDWICH C ROLLING MODEL CONSTANT(K) IF(V.LE.10.0) THEN AK=1.59 ELSE IF(V.LE.45.0) THEN AK=1.40 ELSE IF(V.LE.100.0) THEN AK=1.19 ELSE IF(V.LE.180.0) THEN AK=1.16 ELSE IF(V.LE.250.0) THEN AK=1.12 ELSE WRITE(7,*) "AK IS UNDEFINED" STOP END IF C CALCULATION OF REDUCTION(DEL), PERCENTAGE REDUCTION(DELPER) AND C DEFORMED ROLL RADIUS(DR) DEL = HO-HF DELPER=((HO-HF)/HO)*100 DR = RO*(1+(C*P)/(DEL*W)) C C C

COMPUTATION OF MEAN TEMPERATURE(TMEAN),SURFACE TEMPERATURE(TE), TEMPERATURE DISTRIBUTION(TDIST), MIDDLE TEMPERATURE(TMID) AND TEMPERATURE VARIATION ALONG THICKNESS (T1.....T17)

TMEAN = (TF+(TF/AK))/2.0 TMID = (TMEAN+TF)/2.0 TE = TF/AK TDIST = TMID-TE T(1) =TE DO 7 J=1,4 7 T(J+1) = T(J)+0.2*TDIST DO 8 J=5,7 8 T(J+1) = T(J) +0.04*TDIST T(9) = (TMEAN+TF)/2.0 M=0 DO 9 J=8,5,-1

www.ijesi.org

64 | Page

A Study Of Zenner – Holomon Parameter Variation… M=M+1 9 T(J*2)=T(M*2) M1=3 DO 11 J=15,11,-2 T(J)=T(M1) 11 M1=M1+2 T(17)=T(1) C COMPUTATION OF STRAIN RATE SRT = ((1.08*V)/(DR*DEL)**0.5)*((DEL/(HO*HF))**0.25)*(ALOG(HO/HF) 1)**0.45 C C

ESTIMATION OF THICKNESS VARIATION CORRESPONDING TO TEMPERATURE VARIATION (H1..............H17) ALONG HEIGHT

H(1) = 0 H(2) = HO/17.0 DO 13 J=2,16 IF(J.EQ.8) THEN H(J+1) = HO/2.0 ELSE IF (J.EQ.16) THEN H(J+1) = HO ELSE H(J+1) = H(J)+1 END IF 13 CONTINUE C ESTIMATION OF ZENER HOLLOMON PARAMETER ALONG THICKNESS C (Z1.........Z17) DO 15 J = 1,17 PLOT(J) = ALOG10(SRT*DEXP(Q/(GKR*(T(J)+273)))) 15 CONTINUE

DO 35 J = 1,17 35 AZEN = AZEN+PLOT(J) CONTINUE AZEN = AZEN/17.0 26 FORMAT(1X,'SPECIMEN NO. = 'A4) 27 FORMAT(1X,'MEAN TEMPERATURE,('C) = 'F7.2) 37 FORMAT(1X,'ZENER-HOLLOMON PARAMETER(LOG) = 'F5.2) 40 FORMAT(1X,'ROLLING REDUCTION,(%) = 'F5.2) WRITE(7,26)SPNO WRITE(7,27)TMEAN WRITE(7,40)DELPER WRITE(7,37)AZEN WRITE(7,*)'_____________________________________________' WRITE(*,29)RSM 29 FORMAT(1X,13HEnter, edit ,A14,14Hfor the output) 30 WRITE(*,*)'DO YOU WISH TO CONTINUE?(Y/N)' READ(*,20)CONTD IF(CONTD.EQ.IY) GO TO 10 IF(CONTD.EQ.IN) GO TO 31 WRITE(*,*)'INVALID RESPONSE !! ENTER (Y/N) USING UPPERCASE LETTER' GO TO 30 31 STOP END

www.ijesi.org

65 | Page

A Study Of Zenner – Holomon Parameter Variation… Table I: Chemical Compositions and Thermo-mechanical Data for HCSS316 Element in HCSS316 C S Mo Ni Si Cr W Mn Nb V Ti Co Cu N O

Percentage Composition (%wt) 0.054 0.016 2.050 11.300 0.540 17.400 <0.020 1.370 0.100 0.070 0.040 0.140 0.320 524ppm 122ppm

Preliminary Measurement Mean Grain Size, (m) Aspect Ratio Micro hardness HV (kg/mm2) Temperature, (OC) 0.2% P. S., (N/mm2) Ultimate Tensile Strength, (N/mm2) Elongation, (%) Reduction in Area, (%)

Value 39.30 1.02 165.00 20.00 246.00 595.00 67.00 66.00

TABLE II: The Reverse Sandwich Rolling Experimental Data*. S/N SPEC. FURN. THICKNESS WIDTH ROLLING NO. TEMP. INIT. FINL. SPEED (OC) (mm) (mm) (mm) (mm/s) 1 2 3 4

H50 H51 H52 H53

1120 14.17 12.73 75.17 1128 12.03 10.82 75.20 1123 10.04 09.09 75.20 1122 08.03 07.40 75.23 *(Aiyedun,1984)

009.32 009.32 009.32 009.32

TABLE III: OUTPUT FOR SPECIMEN H50 -------------------------------------SPECIMEN NO. = H50 MEAN TEMPERATURE,('C) = 912.20 ROLLING REDUCTION,(%) = 10.16 ZENER-HOLLOMON PARAMETER(LOG) = 19.66 ______________________________________ TABLE IV: OUTPUT FOR SPECIMEN H51 -------------------------------------SPECIMEN NO. = H51 MEAN TEMPERATURE,('C) = 918.72 ROLLING REDUCTION,(%) = 10.06 ZENER-HOLLOMON PARAMETER(LOG) = 20.76 ______________________________________ TABLE V: OUTPUT FOR SPECIMEN H52 -------------------------------------SPECIMEN NO. = H52 MEAN TEMPERATURE,('C) = 914.64 ROLLING REDUCTION,(%) = 9.46 ZENER-HOLLOMON PARAMETER(LOG) = 20.94 ______________________________________

www.ijesi.org

66 | Page

A Study Of Zenner – Holomon Parameter Variation… TABLE VI: OUTPUT FOR SPECIMEN H53 -------------------------------------SPECIMEN NO. = H53 MEAN TEMPERATURE,('C) = 913.83 ROLLING REDUCTION,(%) = 7.85 ZENER-HOLLOMON PARAMETER(LOG) = 21.02 ______________________________________ Table VII: *Values Obtained for the Specimens Using Sims‟ Theory. S /N

1 2 3 4

Specimen Identification Number H50 H51 H52 H53

Rolling Reduction (%) 10.16 10.06 9.46 7.85

Log10(Z)

19.40 19.60 20.50 21.00

*Shobowale,(1998)

Frictional force

Normal force

Hard Matrix

HO

Soft Clad

Hard Matrix

Hf

Roll

FIG. 1 Schematic Illustration of Reverse Sandwich Rolling Process.

www.ijesi.org

67 | Page

A Study Of Zenner – Holomon Parameter Variation…

START

READ:

SP.NO, V, Tf, H0, W, Hf

NO NO

NO

NO

NO

IS V< 250?

IS V< 180?

IS V< 100?

IS V< 45?

YES

YES

K = 1.59

K = 1.40 COMPUTE

YES

YES

YES

IS V< 10?

K = 1.19

RED = HO - HF % RED = ((HO - HF) /HO))*100 DR = RO*(1+(C*P)/(RED*W)) Tm = (Tf+(Tf / K))/2 TCORE = (TM+ TF)/2 TS = Tf / K TDIST = TCORE - TS 0.25 h1 0.45 1.08V 2 ln 0.5 0.5 R` h1h 2 h 2

K = 1.16

Q LogZ Log exp RT

K = 1.12

COUNTER J = 0 K = UNDEFINED COMPUTE J, T(J), H(J), LogZ NO

YES IS J = 17 ?

J =J+1 NO

NO

ALL SPECIMEN CONSIDERED?

WRITE SP NO,Tm, ,%RED, LogZMEAN

YES

STOP

Fig. 2: Flow Chart for the RSM Simulation

www.ijesi.org

68 | Page

A Study Of Zenner – Holomon Parameter Variation… 21.5

Zener - Hollomon Parameter

21

3

2

y = 0.1367x - 1.28x + 3.9833x + 16.82 R2 = 1

20.5 y = -0.1833x3 + 1.45x2 - 2.8667x + 21 R2 = 1 20

19.5

19 10.16

RSM

SIMS

Poly. (RSM)

Poly. (SIMS)

10.06

9.46

7.85

Rolling Reduction, (%)

FIG.3: DEPENDENCE OF ZENER - HOLLOMON PARAMETER ON ROLLING REDUCTION BASED ON DIFFERENT ROLLING THEORIES

930

925

O

Temperature, ( C)

920

915

910

MEAN; EXPERIMENTAL

MEAN; SIMULATED

905

900 H50

H51

H52

H53

High Carbon Stainless Steel 316 Specimen.

Fig. 4: VALIDATION OF SIMULATED RESULTS USING MEAN ROLLING TEMPERATURE ESTIMATION

www.ijesi.org

69 | Page

Advertisement